SSPC-PA 1 June 1, 2016
SSPC: The Society for Protective Coatings
SSPC-PA 1 SHOP,, FIELD, AND SHOP A ND MAINTENANCE MA INTENANCE COA COATING TING OF O F METALS
3.2 If there is a conict between the requirements of any of the cited reference documents and this standard, the requirements of this standard shall prevail.
1. SCOPE 1.1 This standard provides basic requirements for best practices for application of industrial/marine protective coatings to coated or uncoated metallic substrates, and is intended for use by both speciers and contractors, either in its entirety or by referencing specic sections. It focuses on the coating application process and application-related items that are included as one element of the contractor’s work plan or process control procedures. The scope of this standard includes specic as well as general requirements for the application of liquid coatings applied by brush, spray, or roller. Detailed descriptions of site preparation, surface preparation, pretreatments, or selection of primers and nish coats are beyond the scope of this standard. Appendix A provides additional information about the value and use of project-specic contractor work plans. Appendix B provides an example of language that can be used in procurement/specication documents to specify compliance with requirements of SSPC-PA 1. Appendix C provides a list of additional SSPC reference materials.
3.3 SSPC DOCUMENTS: Determining Compliance to Dry Coating Thickness Requirements Determining Compliance to Steel PA 17 (2012) ProleRequirements Guide 12 (1998) Guide for Illumination of Industrial Painting Projects Guide for Planning Coatings Inspection PA 2 (2015)
3.4 AMERICAN SOCIETY FOR MATERIALS (ASTM) STANDARDS:1
Standard Terminology for Paint, Related Coatings, Materials, and Applications Test Method for Evaluating D660-93 (2011) Standard Test Degree of Checking of Exterior Paints D714-02 (2009) Standard Test Method for Evaluating Degree of Blistering of Paints D4285-83 (2012) (2012) Method for Indicating Oil or Water in Compressed Air Standard Test Method for Measuring E337-15 Humidity with a Psychrometer (the Measurement of Wet- and Dry-Bulb Temperatures) D16 (2014)
2. CONTENTS 1. Scope 2. Contents 3. Referenced Standards 4. Denitions 5. Requirements for Handling and Storage of Coating 6. Requirements to Address Before Coating Application 7. General Requirements for Application of Coatings 8. Requirements for Brush, Roll, and Spray Application 9. Requirements for Shop Coating 10. Requirements for Field Coating 11. Repair of Existing Damaged Coatings 12. Curing and Handling of Applied Coatings 13. Inspection Requirements 14. Disclaimer 15. Notes
3.5 NACE INTERNA INTERNATIONAL TIONAL STANDARD:2 * SP0178 (2007)
Fabrication Details, Surface Finishing Requirements, and Proper Design Considerations for Tanks and Vessels to be Lined for Immersion Service
4. DEFINITIONS BLISTERING: Formation of dome-shaped projections (blisters) in paints or varnish lms resulting from local loss of adhesion and lifting of the lm from an underlying paint lm
3. REFERENCED STANDARDS 3.1 The latest issue, amendment, or revision of the referenced documents in effect at the time of publication of this standard is shown below and shall govern unless otherwise specied. Items preceded by an asterisk asterisk (*) are referenced in the Notes and are not requirements of the standard.
ASTM International, 100 Barr Harbor Drive, West Conshohocken, PA 19428-2959. For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected]
For Annual Book of ASTM Standards volume information, refer to the st andard’s Document Summary page on the ASTM website. NACE International, 15835 Park Ten Place, Houston, Texas 77084. Phone 281-228-6200.
SSPC-PA 1 June 1, 2016
(intercoat blistering) or the base substrate. The standard test method for evaluating the degree of blistering of paints is described in ASTM D 714. CHECKING: Fine cracking that develops in paint lms during prolonged curing or weathering which does not penetrate to the underlying surface. DEFECT: A surface or lm imperfection (aw), deciency, or incompleteness that deviates from a specication or industry-accepted condition. DRIP: A drop of wet coating that forms on or falls from the edge of the coated substrate. DRY SPRAY: A rough, powdery, non-coherent lm produced when an atomized coating partially dries before reaching the intended surface. FIELD COATING: The on-site coating of new or previously coated metallic substrates. HOLD POINT: Critical point in an operation where the processed is stopped until the work completed to date has been evaluated against the project specication or work standard. HOLIDAY: An unintentional void in a coating. INDUCTION TIME: Sometimes called “sweat-in time,” the time interval that must elapse after combining the mixed components of multi-component paint before satisfactory application can begin. MAINTENANCE PAINTING: (1) In broad terms, all painting on industrial structures conducted for protection or aesthetics; (2) Any coating work conducted subsequent to the coating work associated with construction to ensure continuous protection of coated surfaces.
PROCESS CONTROL PROCEDURE: A detailed written description of a process to ensure that it is performed and evaluated consistently. RUNS: Irregularities of a surface due to uneven ow, frequently due to application of a coat that is too heavy and not brushed out well. Also known as “sags” or “curtains.” SAGGING: The irregular downward ow of wet paint under the force of gravity to produce a thicker lower edge . SHOP COATING: The surface preparation and coating of metallic substrates inside a shop or plant before shipment to the site, or when returned to the shop for refurbishment or repair. STRIPE COAT: A coat of paint applied to edges, welds, rivet or bolt heads, nuts, rivets and other irregular surfaces on steel structures before or after a full coat is applied to the entire surface. The stripe coat is intended to give those areas sufcient lm build to resist corrosion. TIE COAT: A coating recommended by the manufacturer of a given paint system that creates an effective chemical or adhesive bond between two coats when the recoat window has been exceeded, or is needed to effect positive adhesion of a coating to a known existing coating sys tem. WORK PLAN: Document containing a list of all actions and procedures that a contractor should perform in logical sequence in order to meet all requirements of the procurement/ specication documents. WRINKLING: A defect that creates small furrows or ridges in a coating lm.
5. REQUIREMENTS FOR HANDLING AND STORAGE OF COATING
MANUFACTURER’S INSTRUCTIONS AND RECOM-
MENDATIONS: These (or similar terms such as Product Data Sheet) are used to refer to an equipment supplier’s or coating manufacturer’s latest published or written instructions and recommendations. Approval of these recommendations shall be obtained from the facility owner or authorized representative. Oral recommendations or instructions from an equipment or coating manufacturer are not acceptable unless backed up in writing by the manufacturer’s technical staff. PAINT: Any pigmented liquid, liqueable, or mastic composition designed for application to a substrate in a thin layer that is converted to an opaque solid lm after application. Used for protection, decoration, identication, or to serve some other functional purposes. PINHOLE: A holiday or discontinuity that extends entirely through a coating lm, approximately the size of a pin; normally caused by solvent bubbling, moisture, or foreign particles . POT LIFE: The length of time during which the mixed coating can be applied after combining two or more components of a multiple-component coating in accordance with the manufacturer’s product data sheet. PRECONSTRUCTION PRIMER: Thin primer coat for steel components, usually applied in a shop prior to construction of a structure, to provide temporary corrosion control during construction. PRETREATMENT: (1) Chemical treatment to prepare a bare metal surface for painting; (2) A wash primer, such as vinyl butyral.
5.1 All coating shall be delivered to the shop or jobsite in original, unopened containers with labels intact. Minor damage to containers is acceptable provided the container has not been punctured or the lid seal broken. The shipment shall be checked upon receipt to verify that: • the correct material has been delivered the product was shipped in accordance with • manufacturer’s shipping requirements all material is from the same batch, unless otherwise • specied 5.2 Each container of coating shall be clearly marked or labeled to show coating identication, date of manufacture, batch number, and other information as needed to meet regulatory requirements. The container label information shall be legible and shall be checked at the time of use to verify that the material’s shelf life has not expired. Each type of coating shall be accompanied by the manufacturer’s Safety Data Sheet (SDS) and product data sheet (PDS). 5.3 Coatings shall be stored in original unopened containers in weather-tight spaces where the temperature is maintained between 40 °F and 100 °F (4 °C and 38 °C) unless otherwise recommended in writing by the manufacturer. The coating temperature shall be brought to the manufacturer’s
SSPC-PA 1 June 1, 2016
written recommended application temperature before use. (See Note 15.1 for more information on coating storage.)
requirements stated in the coating manufacturer’s written recommendations. Unless otherwise specied by the facility owner or authorized representative, the surface cleanliness and prole shall be within the coating manufacturer’s written recommendations for the intended service environment. If the surface to be coated is degraded or contaminated subsequent to surface preparation and prior to coating, the contractor shall verify that the surface has been restored to the specied condition before coating application (see Note 15.2). When veried in accordance with SSPC-PA 17, the surface prole shall be within the prole range appropriate for the coating as specied in the procurement/specication documents, as shown on the product data sheet, or in the manufacturer’s written application instructions.
5.4 Coating shall be used before its shelf life has expired. A coating that has exceeded its shelf life shall not be used unless the contractor or applicator, with permission from the facility owner or authorized representative, has rst obtained a certicate of conformance (COC) from the coating manufacturer. The COC shall verify the acceptability of that batch of coating for use for a specied period of time. 5.5 All containers of coating shall remain unopened until required for use. Coating that has livered, gelled, or otherwise deteriorated during storage shall not be used. Thixotropic materials that are within the viscosity range specied on the product data sheet shall be stirred to attain normal consistency.
6.4.2 Previously applied coating shall be roughened prior to overcoating whenever necessary for the development of proper intercoat adhesion (see Section 7.9). If s pecial surface preparation procedures are required before application of eld coats, the coating manufacturer’s instructions shall be followed.
6. REQUIREMENTS TO ADDRESS BEFORE COATING APPLICATION 6.1 AMBIGUOUS OR CONFLICTING APPLICATION INSTRUCTIONS OR REQUIREMENTS: Items needing clarication such as omissions, discrepancies, apparent errors, or conicting requirements identied in the procurement/ specication documents shall be identied, addressed and resolved prior to beginning the application process. The resolutions shall be documented. See Appendix A for additional information.
6.4.3 Weld Preparation: Before applying the coating, verify that all welds and all areas adjacent to welds meet, at minimum, the cleanliness level and prole range specied for the metallic substrate (see Section 7.4 and Note 15.3). 6.5 REQUIRED AMBIENT CONDITIONS 6.5.1 Temperature: The application of a coating system shall occur only when the air and substrate temperatures are within the ranges indicated by the manufacturer’s written instructions for both application and curing and can be expected to remain in those ranges. Coatings shall not be applied outside the manufacturer’s recommended temperature ranges without the written approval of the manufacturer and the facility owner or authorized representative (see Note 15.4).
6.2 EXEMPT SURFACES: The contractor shall ensure that areas, components and ttings exempt from coating as identied in the procurement/specication documents are noted in any written communication with the application crew. The contractor shall ensure that the areas are protected with materials sufcient to withstand surface preparation and coating operations. If masking instructions are unclear or lacking in the project procurement/specication documents, the contractor shall obtain clarication from the facility owner or authorized representative or those who manage coating projects for the owner or authorized representative. Machine nished or similar surfaces that should not be coated, but do require protection, shall be protected as specied.
6.5.2 Surface Moisture: Unless otherwise specied, or authorized by the facility owner or authorized representative, coating shall not be applied in rain, wind, snow, fog, or mist, or when the metallic substrate’s surface temperature is less than 5 °F (3 °C) above the dew point. Coating shall not be applied to wet or damp surfaces unless the coating is formulated and certied by the manufacturer for this type of application. Coating shall not be applied on frosted or ice-coated surfaces.
6.3 ILLUMINATION: The type of lighting xtures and the level of illumination of the work area shall comply with the minimum requirements listed in SSPC-Guide 12 for the operation being performed (general work area, surface preparation and coating application, or inspection).
6.5.3 Humidity: Because curing of coatings may be adversely affected by humidity that is too low or too high, no coating shall be applied unless the manufacturer’s written recommendations for the humidity range are met (see Note 15.5).
6.4 SURFACE PREPARATION 6.4.1 Immediately prior to coating application, the surface to be coated shall meet the level of cleanliness, surface prole and other surface condition requirements (e.g., grinding of welds and sharp edges) specied in the procurement/specication documents. If surface preparation requirements are not addressed in the procurement/specication documents, the surface shall meet the level of cleanliness and surface prole
6.5.4 Wind Speed: Unless otherwise specied by the facility owner or authorized representative, exterior application of paint shall cease when wind velocity reaches 25 miles per hour or more at the point of application, either in gusts or at a steady state see Note 15.6).
SSPC-PA 1 June 1, 2016
shall be lifted from the bottom of the container with a broad, at paddle. Lumps shall be broken up, and the pigment shall be thoroughly mixed with the remaining vehicle. The poured-off vehicle shall be returned to the coating with simultaneous stirring, until the composition is uniform.
6.6 PROTECTION OF EXPOSED SUBSTRATE FROM WEATHER: If ambient conditions are not suitable for coating application, the metallic substrate shall remain under cover or be protected by enclosure in containment until ambient conditions permit coating application to proceed.
18.104.22.168 Power Mixing: Power mixing of single-component materials is permitted unless otherwise recommended in product data sheets. Power mixing shall be carried out with a suitable high-torque variable-speed mixer at a sufcient speed to blend the materials. The agitator blade shall be capable of lifting material that dropped out of suspension off the bott om of the container. Care shall be taken to limit the speed to ensure that there is no entrainment or entrapment of air in the coating while ensuring that the blending action is suitable. Mixed coating shall not show evidence of air entrapment. Mixing of solvent-containing coatings in open containers shall be done in a ventilated area away from sparks or ames in accordance with applicable safety regulations.
6.7 REQUIRED PRETREATMENT 6.7.1 When specied, the surface shall be pretreated prior to application of the prime coat. The pretreatment shall be compatible with the specied primer as documented by the coating manufacturer. 6.7.2 The provisions of Section 5 and Section 6.4 shall also apply to pretreated surfaces and the materials used for this purpose. 6.7.3 In order to control the degradation or contamination of cleaned surfaces, the pretreatments, or, in the absence of a pretreatment, the prime coat, shall be applied as soon as possible after the surface has been cleaned and before degradation or contamination has occurred. Succeeding coats shall be applied before contamination of any existing coating occurs.
6.8.3 Where a skin has formed in the container, the skin shall be cut loose from the sides of the container, removed and discarded. If the volume of such skins is visually estimated to be more than 2% of the remaining coating, the coating shall not be used.
6.7.4 When chemical pretreatments are specied, s ufcient time shall elapse between pretreatment and application of the prime coat to permit any chemical reactions to be completed and the surface to dry. Multi-component pretreatments shall be applied within the specied interval after mixing. When pretreatments are used, the instructions of the pretreatment manufacturer shall be followed.
6.8.4 Coating shall not be mixed or kept in suspension by means of an air stream bubbling under the coating surface. 6.8.5 Dry pigments that are separately packaged shall be mixed into coatings in such a manner that they are uniformly blended and all particles of the dry powder are wetted by the vehicle.
6.7.5 Inhibitive water washes used to prevent rusting of cleaned surfaces prior to coating shall not be considered pretreatments. These shall be used only as specied and only if it is documented by the coating manufacturer that the inhibitor is compatible with the coating to be used and will not have adverse long-term effects on the performance of the coating. When specied, test patches shall be used to check adhesion of the coating prior to coating the entire surface.
6.8.6 Multiple-component coatings shall be mixed in the correct proportions in accordance with the coating manufacturer’s written recommendations. Proper mix ratio shall be maintained when mixing multi-component coatings to ensure that they are blended properly and achieve a proper cure. 6.8.7 Coating materials shall be pre-mixed prior to catalyzing or introduction into equipment to ensure that the material is homogeneous and all the solids are properly dispersed.
6.8 MIXING OF COATING COMPONENTS 6.8.1 Manual mixing shall be limited to mixing/blending of low-viscosity single-component coatings. The coating shall be blended completely to ensure that all elements of the materials are suspended properly in the coating (see Note 15.7). Coating shall be strained or ltered after mixing according to the manufacturer’s recommendations, except where application equipment is provided with strainers. Strainers shall be of a size to remove skins and undesirable matter, but not to remove the pigment.
6.8.8 Catalysts, curing agents, or hardeners that are separately packaged shall be added to the base coating only after the latter has been thoroughly mixed. The proper volume of the catalyst shall then be slowly poured into the required volume of base with constant agitation. To avoid mixing incorrect ratios of components, mix only compl ete kits. Do not pour off liquid that has separated from the pigment and then add the catalyst to the settled pigment to aid mixing. The mixture shall be used within the pot life specied by the manufacturer. Therefore, only enough coating shall be catalyzed for prompt use. Most mixed, catalyzed coatings cannot be stored, and unused portions of these shall be placed in proper storage containers for later appropriate disposal (see Note 15.8).
6.8.2 The following are acceptable methods for mixing most single-component coatings: 22.214.171.124 Manual (Hand) Mixing: Most of the vehicle shall be poured off into a clean container. The pigment in the coating 4
SSPC-PA 1 June 1, 2016
When specied, special continuous mixing equipment shall be used according to the manufacturer ’s directions.
shall be thoroughly mixed separately before combining and further mixing. For multiple components, similar components of the two different colors shall be blended together before combining and mixing these blends.
6.8.9 Pastes shall be made into coatings in such a manner that the paste shall be uniformly blended and all lumps and particles broken up to form a homogenous coating.
7. GENERAL REQUIREMENTS FOR APPLICATION OF COATINGS
6.8.10 Coating that does not have a limited pot life or does not deteriorate on standing may be mixed at any time before using, but if settling or phase separation has occurred it must be remixed immediately before using.
7.1 GENERAL: Coating shall be applied in accordance with the manufacturer’s written instructions and the project specication. If there is a conict between the requirements of the manufacturer and the project specication, the more restrictive requirements shall be used unless an exception is approved by the facility owner or authorized representative prior to beginning the application process.
6.8.11 Coating shall not remain in spray pots, painters’ buckets, etc., overnight, but shall be stored in a covered container and remixed before use. 6.9 MANUFACTURER’S REQUIRED INDUCTION TIME
7.2 NUMBER OF COATS AND TYPE OF COATING: The number of coats, type of coat ing, and surfaces to be coated are normally specied in the procurement/specication documents. If coating thickness is not specied, the dry lm thickness (DFT) shall comply with the coating manufacturer’s written recommendations. The coating application shall be scheduled to provide protection to the substrate at all construction stages (see Notes 15.10 and 15.11).
AND POT LIFE: The induction time (sometimes called “sweat-in time”) and pot life stated on the coating manufacturer’s product data sheet must be observed. 6.10 THINNING 6.10.1 Thinning of the coating shall be done in accordance with the manufacturer’s product data sheet and only with the approval of the facility owner or authorized representative (see Note 15.9). The use of thinners shall comply with air pollution control regulations. In no case shall more thinner be added than that recommended by the manufacturer ’s written instructions.
7.3 STRIPE COAT APPLICATION: When stripe coating is specied in the procurement/specication documents, all corners, crevices, rivets, nuts, bolts, welds, and sharp edges shall be stripe coated. Unless otherwise specied or approved by the facility owner, the stripe coat shall be applied by brush before applying a full coat. The stripe coat shall extend a minimum of one inch (2 cm) from the edge it is protecting. The coating manufacturer’s recommended recoat windows for the stripe coat and full coat shall be observed (see Note 15.12).
6.10.2 The type and amount of thinner added to the coating shall be in accordance with the coating manufacturer’s product data sheets for the specic coating being applied, the prevailing ambient conditions and surface temperature, and local air pollution regulations.
7.4 APPLICATION NEAR AREAS TO BE WELDED: If the coating specied can be damaged by the heat of welding, or will create fumes hazardous to the welder when heated during the welding process, or is detrimental to the welding operation or the nished welds, the metallic substrate shall not be coated within four inches (100 millimeters) of the areas to be welded, except when using inorganic zinc-rich primer, which may be applied to within two inches (50 millimeters) of the weld area.
6.10.3 When the use of thinner is permissible, thinner shall be added slowly to the coating during the mixing process. For multi-component coatings, thinner is added to the binder during the mixing process. All thinning shall be done under supervision of a knowledgeable person acquainted with the correct amount and type of thinner to be added to the coating and familiar with pertinent regulations relating to solvent emissions.
7.5 APPLICATION CONTINUITY: To the maximum extent practical, each coat shall be applied as a visually continuous lm of uniform thickness free of holidays, pinholes, and other defects (including runs, drips, sags, etc.). All thin spots or areas missed in the application shall be recoated and permitted to dry before the next coat of coating is applied.
6.11 TINTING: When successive coats of coating of the same color have been specied, alternate coats of coating shall be tinted, when practical, to produce enough contrast to indicate complete coverage of the surface. Tinting shall be performed in such a manner that it will not be necessary to tint the nal coat. Field tinting shall be done only with coatings of the same type from the same manufacturer. When the coating is the color of the metallic substrate, the rst coat to be applied shall be tinted. The tinting material shall be c ompatible with the coating and not detrimental to its service life. It is suggested that the coating be tinted by the manufacturer and appropriately labeled. Single component coatings to be blended for tinting
7.6 DRY FILM THICKNESS (DFT): Unless otherwise specied in the procurement/specication documents, all dry lm thickness determinations shall be performed as specied in SSPC-PA 2. If no Coating Thickness Restriction Level is specied, Level 3 shall be the default level.
SSPC-PA 1 June 1, 2016
7.6.1 If not otherwise specied, each applied coat shall be within the range specied for that coat by the product data sheet or procurement/specication documents.
7.9 INACCESSIBLE AREAS: Metallic surfaces that will be inaccessible for coating after assembly or eld erection shall receive the full specied coating system before assembly or erection.
7.6.2 In the event the required minimum thickness is not achieved as specied, additional coats shall be applied in accordance with the procurement/specication documents or the coating manufacturer’s instructions until the required thickness is obtained. Inorganic zinc-rich coatings shall not be corrected in this manner unless the manufacturer’s instructions specically permit this practice.
7.10 PROTECTION OF COATED SURFACES: Wet coating shall be protected against damage from dust or other detrimental foreign matter as much as is practical.
8. REQUIREMENTS FOR BRUSH, ROLL, AND SPRAY APPLICATION 8.1 GENERAL: Apply the coatings using the application methods recommended by the coating manufacturer and as approved by the facility owner or authorized representative (see Notes 15.14 and 15.15). If a conict arises between the application recommendations in the product data sheet and those in the procurement/specication documents, the contractor or applicator shall seek written clarication from the owner or authorized representative. This standard contains requirements for application using the most common application methods. Specialized methods such as plural-component spray, dipping, ow coating, electrostatic spray, and uidized bed application shall be performed by craft workers who have been properly qualied and trained for specialized equipment and application techniques. Whichever application method is used, the dry lm thickness of each coat shall meet the requirement of the procurement/specication documents. If no requirements are provided in the procurement/specication documents, the dry lm thickness of each coat shall meet the recommended range on the product data sheet for that coating.
7.7 RECOAT WINDOWS: Each coating layer shall be in a proper state of cure or dryness before the application of the succeeding coat so that it is not adversely affected by topcoating. Consult the coating manufacturer for the appropriate time interval before recoating. When applying multiple coats of two-component thermosetting systems, topcoats shall be applied within the recoat window specied by the manufacturer of the undercoat in order to obtain good intercoat adhesion. If, for any reason, this time period is exceeded, the undercoat surface shall be treated as recommended by its manufacturer before topcoating. Such treatments include mild abrasion, solvent treatment, and use of a tie coat. Remove surface contamination that could affect the adhesion of subsequent coats. 7.8 CONTACT SURFACES: Contact surfaces shall be coated or left uncoated as specied in the procurement/ specication documents. 7.8.1 Contact surfaces of members to be joined by high strength bolts in a friction connection (faying surfaces) shall provide the required slip coefcient based on the specied class of slip resistance based on the design criteria. Uncoated faying surfaces shall meet the surface preparation and cleanliness requirements for the specied class and shall be free of oil and grease. If coated faying surfaces are required or permitted, the coating used shall be tested and certied to the required class (see Note 15.13) and shall not exceed the allowable thickness as stated on the Certication. If the coating is thinned, the manufacturer and type of thinner shall be the same type as stated on the Test Certicate. The amount of thinner used should be the same as stated on the Test Certicate; however greater or lesser amounts of thinner may be necessary for proper atomization. The maximum amount of thinner added shall not exceed the manufacturer’s instructions. The application to, or removal of, coating from bolt hole interiors is not required unless specied in procurement/specication documents, although overspray coating is frequently present.
8.2 BRUSH APPLICATION: Brush application of coating shall be in accordance with the following: 8.2.1 Brushes shall be of a style and quality that will enable proper application of coating. 8.2.2 The brushing shall be done so that a smooth coat as uniform in thickness as possible is obtained. 8.2.3 Coating shall be worked into all crevices and corners. 8.2.4 All runs or sags shall be brushed out immediately. 8.2.5 Brush marks and other surface irregularities shall be minimized. 8.3 ROLLER APPLICATION: Roller application shall be in accordance with the following:
7.8.2 Coatings on metallic substrates to be embedded, encased or completely enclosed in concrete shall be compatible with concrete.
8.3.1 Rolling shall be done so that a smooth coat as uniform in thickness as possible is achieved (see Note 15.16). 8.3.2 Roller covers that do not shed bers into the paint shall be used. The roller cover nap shall be appropriate for the particular surface roughness.
7.8.3 The areas to be in contact with wood shall receive the full specied coating system before assembly.
You're Reading a Preview Unlock full access with a free trial.
Download With Free Trial
SSPC-PA 1 June 1, 2016
accordance with the coating manufacturer’s recommended procedures and shall be approved by the facility owner or authorized representative.
10.4.2 Application of Field Coat: The rst eld coat shall be applied to shop-coated metallic substrates in a timely manner, as required by the project procurement/specication documents, to protect the metallic substrate from corrosion and to comply with any applicable rec oat window for the shopapplied coating. SSPC surface preparation standards require the metallic surface to meet specied cleanliness requirements immediately prior to coating application.
9. REQUIREMENTS FOR SHOP COATING 9.1 APPLICABILITY: All provisions of this standard shall be applicable to shop coating except those under Section 10.
10.4.3 The nal coat of coating shall not be applied to metallic substrates until all concrete work in the vicinity is nished. In addition to the cleaning required in Section 10.4.1, all concrete spatter and drippings shall be removed from the metallic substrate before any application of coating. If any coating is damaged due to concrete work, the damaged surface shall be cleaned and recoated before the nal coat is applied.
9.2 TOUCH-UP OF SHOP COATED SURFACES: Damage resulting from fabrication, handling, and storage in the shop shall be repaired before leaving the shop. Metal that has been shop-coated shall be touched up with the same coating as the shop coat unless otherwise specied. Inorganic zinc-rich coatings shall not be corrected in this manner unless the manufacturer’s instructions specically permit this practice. 9.3 ERECTION MARKS: Erection and weight marks that need to be visible after erection shall be placed over cured shop-applied coatings unless otherwise specied. Compatible and non-bleeding markers or coating sticks shall be used.
11. REPAIR OF EXISTING DAMAGED COATINGS 11.1 SURFACE PREPARATION FOR RECOATING 11.1.1 Only loose, cracked, brittle, or non-adherent coating shall be removed in cleaning unless otherwise specied. Cleaning shall be performed two inches (50 millimeters) beyond the damaged areas in all directions or until only sound coating remains in the area to be repaired. Where the remaining coating is thick, all exposed edges shall be feathered. Rust spots shall be thoroughly cleaned and the edges of all old coating shall be abraded back to sound material (see Note 15.20).
10. REQUIREMENTS FOR FIELD COATING 10.1 APPLICABILITY: All provisions of this standard shall pertain to the eld coating of metallic substrates except those in Section 9. 10.2 CURE: Previously applied shop coatings shall be dry or cured sufciently for overcoating and shall meet project procurement/specication requirements for surface cleanliness and roughening. The manufacturer’s instructions shall be followed if special surface preparation procedures are required before application of the eld coats.
11.1.2 The contractor shall have the option to remove all coating from large areas containing smaller areas of coating that are required to be removed by the procurement/specication documents.
10.3 COATING COMPATIBILITY: If the eld coatings are not specied, the coatings selected shall be compatible with the shop coating and the service environment as determined by the primer manufacturer.
11.2 INCOMPATIBILITY: Only coatings compatible with the existing coatings and the service environment shall be used. All defects arising from unexpected incompatibility shall be corrected as specied.
10.4 FIELD COATING PROCEDURES
12. CURING AND HANDLING OF APPLIED COATINGS
10.4.1 Touch-Up of Shop Coated Surfaces: Metallic substrates stored pending erection shall be kept free from contact with the ground and positioned to minimize waterholding pockets, soiling, contamination, and deterioration of the coating lm. Metallic substrates shall be cleaned and recoated or touched up with the specied coating whenever it becomes necessary to maintain the integrity of the lm. Metal that has been shop coated shall be touched up with the same coating as the shop coat unless otherwise specied. Inorganic zinc-rich coatings shall not be corrected in this manner unless the manufacturer’s instructions specically permit this practice. This touch-up shall include preparing, cleaning and coating of eld connections, welds or fasteners, and all damaged or defective coating and rusted areas as specied.
12.1 CURING OF COATINGS 12.1.1 The ambient temperature and humidity as well as minimum and maximum curing times shall conform to manufacturer’s written recommendations prior to topcoating. If the maximum cure time is exceeded, the cured coating shall be roughened or otherwise treated as recommended by the manufacturer of the topcoat or overcoat before applying another coat. 12.1.2 No coating shall be force-cured under conditions that will cause checking, wrinkling, blistering, formation of pinholes, or detrimentally affect the protective properties of the coating. Always check with the coating manufacturer before force-curing a coating.
SSPC-PA 1 June 1, 2016
12.1.3 Coating shall be protected from rain, condensation, contamination, snow, and freezing until sufciently cured for exterior exposure.
easier and thinning the coating prior to application can be avoided. When warming coatings, their temperature should not be permitted to exceed 100 °F (38 °C) unless special coating heating equipment is used. When the coating (or thinner) has a ash point below 100 °F (38 °C) it should not be heated above its ash point if it is heated in an open container.
12.1.4 No coating shall be subjected to immersion before it is thoroughly cured in accordance with the manufacturer’s written recommendations.
15.2 Overcoating should be accomplished as soon as possible after curing requirements of undercoats are met. When this is not feasible, the surface should be restored to the cleanliness level required for application of the overcoat. This may require washing or solvent cleaning of the surface to remove soluble contaminants or, if rusting or damage to the coating has occurred, power tool cleaning or blast cleaning and spot repair may be necessary.
12.2 HANDLING OF COATED METALLIC SUBSTRATES 12.2.1 Coated metallic substrates shall not be handled, loaded for shipment, or shipped until the coating has dried except as necessary in turning for coating or stacking for drying. 12.2.2 Coating that is damaged in handling shall be removed and touched up with the same number of coats and kinds of coatings as were previously applied to the metallic substrate or as specied by the procurement/specication documents.
15.3 Options for cleaning welds include blast cleaning, power tool cleaning, chemical scrubbing, or water scrubbing to remove detrimental deposits. Chemical or water scrubbing will not provide a prole on the weld. The procurement/ specication documents should contain requirements for surface preparation cleanliness level and cleaning method. For high-performance coating service, special weld surfacing may be required to provide suitable surface conditions for the coating system specied. NACE SP0178 provides one method of specifying weld surfacing requirements, as well as other design and fabrication requirements for improving coating serviceability. Other methods of specifying and accepting weld surfacing conditions are employed in various industries. The weld surfacing requirements are generally placed in the procurement/specication documents so that the painting contractor will not have to perform welding or grinding to provide the specied nal surface conditions.
13. INSPECTION REQUIREMENTS The contractor’s work plan (or the inspector’s inspection plan) shall include hold points prior to each step of the application as described in the SSPC Guide for Planning Coating Inspection (2008). These include: Pre-surface preparation Post-surface preparation Coating conditions for application Coating application Post-application of coating Post-curing
15.4 Cold weather, high humidity, water, fog and mist, and rain during coating application, drying, or curing are detrimental to the performance of most coatings. It is impossible to set down specic rules that govern the limits in which the coating application should be done, since the variation from one coating to another may be large. Generally speaking, application should be done only under conditions that are conducive to quick evaporation of water. This generally means that the relative humidity needs to be low. Metallic substrates should not be coated when it is below the dew point since condensation of water on the metallic substrate will result. The only exception is for coatings that are formulated to tolerate moisture or liquid water on the surface during application Coatings that dry solely by evaporation of organic solvent are not normally harmed by application to metallic substrates which are below 32 °F (0 °C); however, under such conditions, the danger always exists that there will be a layer of ice on the surface of the metallic substrate. This same condition may prevail for application of conventional, air-oxidizing coatings. When the humidity is low and the metallic substrate is thoroughly dry, coatings may be applied provided they will not be damaged and that drying will not be impaired by low temperature or low humidity.
14. DISCLAIMER 14.1 This is a consensus standard developed by SSPC: The Society for Protective Coatings. While every precaution is taken to ensure that all information furnished in SSPC standards standard is as accurate, complete, and useful as possible, SSPC cannot assume responsibility nor incur any obligation resulting from the use of any materials, coatings, or methods specied herein, or of the standard itself. 14.2 This standard does not attempt to address problems concerning safety associated with its use. The user of this standard, as well as the user of all products or practices described herein, is responsible for instituting appropriate health and safety practices and for ensuring compliance with all governmental regulations.
15. NOTES Notes are not requirements of this standard. 15.1 It is recommended that coating be stored in a warm building during very cold weather because application will be 9
SSPC-PA 1 June 1, 2016
Generally speaking, coatings should not be applied when ambient conditions will subject them to damage, nor should they be applied when it is expected that the temperature will vary either below or above the temperature range recommended in writing by the manufacturer or drop to freezing before they have cured. Coatings formulated for application to hot surfaces may not be suitable for application to surfaces below the designed temperature. Conversely, coatings formulated for application at ambient or low temperatures may not be suitable for application to hot surfaces. Low temperatures greatly reduce the curing rates of chemically cured coatings (certain epoxies, urethanes, inorganic zinc-rich coatings, coal tar epoxies, etc.). The dew point is the temperature at which moisture from the air will begin to condense. If the surface temperature of the substrate is at the dew point, moisture will condense on it. Dew point may be determined with a sling psychrometer, or other instrument, usually requiring determination of wet and dry bulb temperatures (ASTM E337). Hand-held, digital psychrometers, hygrometers, etc., can make measurement of relative humidity and dew point simple and instantaneous. These electronic instruments can alsomeasure of relative humidity and dew point of a surface that is at a different temperature than the air.
Particular care should be observed with respect to type of thinner, amount of thinner, coating temperature, and operating techniques in order to avoid deposition of coating which is too viscous, too dry, or too thin. At very low temperatures, thinners can shock sensitive coating materials, resulting in gelling. It may be necessary to use an approved different coating material or other equipment to resolve these problems. 15.10 Preconstruction primers are usually formulated to provide short-term protection and a good bond between the metallic substrate and subsequent coats. Many preconstruction primers are not intended to provide long-term protection of the metallic substrate, particularly during exposure to dampness, bad weather, and industrial fumes. Between shop application of the primer and eld coating application, the metallic substrate is often exposed to the most severe environmental conditions it will ever encounter at a time when it is protected by only one coat of primer. The length of time anticipated between shop application of the primer and the rst eld-applied coating should be considered when selecting the primer to be used. Long periods of eld exposure may degrade the primer so that it may have to receive periodic maintenance to continue to protect the metallic substrate from corrosion and be in a suitable condition for overcoating. When long periods of exposure are anticipated, special consideration should be given to surface preparation, coating selection, lm thickness, and to early application of a second primer/overcoat.
15.5 High humidity may cause moisture to condense on or react with uncured coating lms to cause blushing or other adverse effects. However, some coatings such as inorganic zinc and moisture-cured urethane coatings cure by chemically reacting with water, and so require a minimum humidity for complete curing.
15.11 Whenever possible, the last full (nish) coat of coating should be applied after erection of the structure and repair of damaged areas of existing coating. Members may be coated on the ground before erection, provided any damaged coating is touched-up with the same number of coats and kinds of coatings after erection.
15.6 The project specications may address maximum wind velocity permissible during coating application. A lower velocity may be specied due to individual jobsite conditions and associated safety concerns.
15.12 Stripe coating of edges, corners, fasteners, welds, etc., is advantageous in preventing breakdown of coating on such congurations in very corrosive surroundings. Stripe coating is most effective on edges that are prepared by grinding. Tinting of the striping coating is advisable to promote contrast (see Section 7.3). Additional information on stripe coating and edge protection is available in SSPC-PA Guide 11.
15.7 Power mixing of the components of the coating is preferable to manual (hand) mixing due to the higher viscosity of materials in industrial coatings, particularly where multi-component materials are used. Pigments or solids that inadvertently are not mixed back into the coating may adversely affect the performance of the coating. The coating manufacturer should be consulted for acceptable mixing tolerances.
15.13 The Specication for Structural Joints Using HighStrength Bolts, published by the Research Council on Structural Connections (RCSC), includes a procedure for determining the slip coefcient of a coating. Most facility ownersthat have been certied to meet the appropriate slip coefcient requirements. 3
15.8 Mixing of some coating components can cause a chemical reaction called an “exothermic reaction,” generating heat that can result in expansion of the materials, and a release of vapors or gases that may rupture sealed containers. If exothermic reaction is a possibility, the containers should be vented.
15.14 There may be limitations on application techniques based on location and conguration of the facility. For example, spray application may be restricted due to the potential for overspray damage on adjacent surfaces.
15.9 Coatings to be applied by brush will usually require no thinning. Coatings to be sprayed, if not specically formulated for spraying, may require thinning when proper adjustment of the spray equipment and air pressure does not result in satisfactory coating application.
American Institute of Steel Construction Research Council on Structural Connections, One East Wacker Drive, Suite 700, Chicago, IL 60601-1802. Phone 312-670-5414,